In this study, various properties of hydrogel are controlled at various levels while maintaining their intrinsic properties to meet the specific requirements.
In chapter 2, While maintaining the intrinsic properties of PEG hydrogels, a mechanism for effectively controlling drug release kinetics was provided. By presenting pendant PEG chains with characteristic end functional groups in PEG hydrogels, their various physical properties (i.e., charge density and hydrophobicity) effectively controlled the release of proteins with different isoelectric points (pI) independent of the crosslinking density.
In chapter 3, The mechanical properties and decomposition behavior of PEGDA-PEI hydrogels prepared by in situ crosslinking between PEGDA and PEI via Michael addition were investigated by varying the MW and concentration. This combination of tunable mechanical properties and degradation behavior of PEGDA-PEI hydrogels was highly effective in controlling the rate and mode of drug release by dual-mode drug release mechanisms.
In chapter 4, in situ formation chitosan hydrogels via Schiff base formation controlled a wide range of mechanical properties without compromising gelation kinetics. Chitosan was conjugated with PEG grafts with controlled length and density (PEG-g-Cs), allowing water solubility at physiological pH, as well as directly affecting the mechanical results of the resulting Cs-PEG hydrogel. The adhesive properties and clinical potential of Cs-hydrogels was evaluated by ex vivo and in vivo model, which showed wound closure with minimal inflammation with similar mechanical properties as commercial tissue sealants.
In chapter 5, By inducing the formation of Schiff bases between aldehyde-presented alginate (Alg- ALD) and amine-presented polyasparmide, an in situ formation and rapid decomposition hydrogel system was developed. The potential of Alg-PHEA hydrogels as a tissue injectable delivery system was demonstrated ex vivo, in which hydrogel could be stably formed within the tissue upon injection, gradually degraded over time, and eventually completely dissolved. Moreover, their degradation rate and complete dissolution could be further modulated by additional ionic cross-linking of alginate.
Through the development of in situ crosslinked hydrogels with controllable properties by varying the graft architecture and the modulation of the mechanical and physicochemical properties of hydrogels for refined drug release kinetics, the clinical application of hydrogels has been demonstrated in both in vitro and in vivo models. Therefore, by developing versatile hydrogels, it is expected to increase their potential use in biomedical fields.
1. Mondal, S., S. Das, and A.K. Nandi, A review on recent advances in polymer and peptide hydrogels. Soft Matter, 2020. 16(6): p. 1404-1454.
2. Caló, E. and V.V. Khutoryanskiy, Biomedical applications of hydrogels: A review of patents and commercial products. European Polymer Journal, 2015. 65: p. 252-267.
3. Ahmed, E.M., Hydrogel: Preparation, characterization, and applications: A review. Journal of Advanced Research, 2015. 6(2): p. 105-121.
4. Hu, W., et al., Advances in crosslinking strategies of biomedical hydrogels. Biomaterials Science, 2019. 7(3): p. 843-855.
5. Yang, J.-A., et al., In situ-forming injectable hydrogels for regenerative medicine. Progress in Polymer Science, 2014. 39(12): p. 1973-1986.
6. Choi, B., et al., Introduction to In Situ Forming Hydrogels for Biomedical Applications, in In- Situ Gelling Polymers: For Biomedical Applications, X.J. Loh, Editor. 2015, Springer Singapore: Singapore. p. 5-35.
7. Vermonden, T., R. Censi, and W.E. Hennink, Hydrogels for Protein Delivery. Chemical Reviews, 2012. 112(5): p. 2853-2888.
8. Wang, C., R.R. Varshney, and D.-A. Wang, Therapeutic cell delivery and fate control in hydrogels and hydrogel hybrids. Advanced Drug Delivery Reviews, 2010. 62(7): p. 699-710.
9. Drury, J.L. and D.J. Mooney, Hydrogels for tissue engineering: scaffold design variables and applications. Biomaterials, 2003. 24(24): p. 4337-4351.
10. Schmidt, J.J., J. Rowley, and H.J. Kong, Hydrogels used for cell-based drug delivery. Journal of Biomedical Materials Research Part A, 2008. 87A(4): p. 1113-1122.
11. Ruoslahti, E., RGD AND OTHER RECOGNITION SEQUENCES FOR INTEGRINS. Annual Review of Cell and Developmental Biology, 1996. 12(1): p. 697-715.
12. Zhu, J., Bioactive modification of poly(ethylene glycol) hydrogels for tissue engineering.
Biomaterials, 2010. 31(17): p. 4639-4656.
13. Lin, C.-C. and K.S. Anseth, PEG Hydrogels for the Controlled Release of Biomolecules in Regenerative Medicine. Pharmaceutical Research, 2009. 26(3): p. 631-643.
14. Weber, L.M., C.G. Lopez, and K.S. Anseth, Effects of PEG hydrogel crosslinking density on protein diffusion and encapsulated islet survival and function. Journal of Biomedical Materials Research Part A, 2009. 90A(3): p. 720-729.
15. Hoare, T.R. and D.S. Kohane, Hydrogels in drug delivery: Progress and challenges. Polymer, 2008. 49(8): p. 1993-2007.
16. Anseth, K.S., C.N. Bowman, and L. Brannon-Peppas, Mechanical properties of hydrogels and their experimental determination. Biomaterials, 1996. 17(17): p. 1647-1657.
17. Cha, C., et al., Decoupled control of stiffness and permeability with a cell-encapsulating poly(ethylene glycol) dimethacrylate hydrogel. Biomaterials, 2010. 31(18): p. 4864-4871.
18. Cruise, G.M., D.S. Scharp, and J.A. Hubbell, Characterization of permeability and network structure of interfacially photopolymerized poly(ethylene glycol) diacrylate hydrogels.
Biomaterials, 1998. 19(14): p. 1287-1294.
19. Fefelova, N.A., et al., Mucoadhesive interactions of amphiphilic cationic copolymers based on [2-(methacryloyloxy)ethyl]trimethylammonium chloride. International Journal of Pharmaceutics, 2007. 339(1): p. 25-32.
20. Huynh, D.P., et al., Controlled release of insulin from pH/temperature-sensitive injectable pentablock copolymer hydrogel. Journal of Controlled Release, 2009. 137(1): p. 20-24.
21. Lee, W.-F. and P.-L. Yeh, Thermoreversible hydrogels. VIII. Effect of a zwitterionic monomer on swelling behaviors of thermosensitive hydrogels copolymerized by N-isopropylacrylamide with N,N′-dimethyl (acrylamidopropyl) ammonium propane sulfonate. Journal of Applied Polymer Science, 1999. 74(9): p. 2170-2180.
22. Matsusaki, M. and M. Akashi, Novel Functional Biodegradable Polymer IV: pH-Sensitive Controlled Release of Fibroblast Growth Factor-2 from a Poly(γ-glutamic acid)-Sulfonate Matrix for Tissue Engineering. Biomacromolecules, 2005. 6(6): p. 3351-3356.
23. Vinogradov, S.V., T.K. Bronich, and A.V. Kabanov, Nanosized cationic hydrogels for drug delivery: preparation, properties and interactions with cells. Advanced Drug Delivery Reviews, 2002. 54(1): p. 135-147.
24. Yu, L., Z. Zhang, and J. Ding, In vitro degradation and protein release of transparent and opaque physical hydrogels of block copolymers at body temperature. Macromolecular Research, 2012. 20(3): p. 234-243.
25. Bae, M.S., et al., Development of novel photopolymerizable hyaluronic acid/heparin-based hydrogel scaffolds with a controlled release of growth factors for enhanced bone regeneration.
Macromolecular Research, 2016. 24(9): p. 829-837.
26. Kim, S., K. Lee, and C. Cha, Refined control of thermoresponsive swelling/deswelling and drug release properties of poly(N-isopropylacrylamide) hydrogels using hydrophilic polymer crosslinkers. Journal of Biomaterials Science, Polymer Edition, 2016. 27(17): p. 1698-1711.
27. Akiyama, Y., Y. Nagasaki, and K. Kataoka, Synthesis of Heterotelechelic Poly(ethylene glycol) Derivatives Having α-Benzaldehyde and ω-Pyridyl Disulfide Groups by Ring Opening Polymerization of Ethylene Oxide Using 4-(Diethoxymethyl)benzyl Alkoxide as a Novel Initiator. Bioconjugate Chemistry, 2004. 15(2): p. 424-427.
28. Cammas, S., Y. Nagasaki, and K. Kataoka, Heterobifunctional Poly(ethylene oxide): Synthesis of .alpha.-Methoxy-.omega.-amino and .alpha.-Hydroxy-.omega.-amino PEOs with the Same Molecular Weights. Bioconjugate Chemistry, 1995. 6(2): p. 226-230.
29. Jang, J., J. Hong, and C. Cha, Effects of precursor composition and mode of crosslinking on mechanical properties of graphene oxide reinforced composite hydrogels. Journal of the Mechanical Behavior of Biomedical Materials, 2017. 69: p. 282-293.
30. Cha, C., R.H. Kohman, and H. Kong, Biodegradable Polymer Crosslinker: Independent Control of Stiffness, Toughness, and Hydrogel Degradation Rate. Advanced Functional Materials, 2009. 19(19): p. 3056-3062.
31. Kim, S., et al., Comprehensive Examination of Mechanical and Diffusional Effects on Cell Behavior Using a Decoupled 3D Hydrogel System. Macromolecular Bioscience, 2017. 17(9):
32. Cha, C., J.H. Jeong, and H. Kong, Poly(ethylene glycol)-poly(lactic-co-glycolic acid) core–
shell microspheres with enhanced controllability of drug encapsulation and release rate.
Journal of Biomaterials Science, Polymer Edition, 2015. 26(13): p. 828-840.
33. Ferrero, C., D. Massuelle, and E. Doelker, Towards elucidation of the drug release mechanism from compressed hydrophilic matrices made of cellulose ethers. II. Evaluation of a possible swelling-controlled drug release mechanism using dimensionless analysis. Journal of Controlled Release, 2010. 141(2): p. 223-233.
34. Fu, Y. and W.J. Kao, Drug release kinetics and transport mechanisms of non-degradable and degradable polymeric delivery systems. Expert Opinion on Drug Delivery, 2010. 7(4): p. 429- 444.
35. Siepmann, J. and N.A. Peppas, Modeling of drug release from delivery systems based on hydroxypropyl methylcellulose (HPMC). Advanced Drug Delivery Reviews, 2012. 64: p. 163- 174.
36. Zustiak, S.P. and J.B. Leach, Hydrolytically Degradable Poly(Ethylene Glycol) Hydrogel Scaffolds with Tunable Degradation and Mechanical Properties. Biomacromolecules, 2010.
11(5): p. 1348-1357.
37. Peppas, N.A., et al., Poly(ethylene glycol)-containing hydrogels in drug delivery. Journal of Controlled Release, 1999. 62(1): p. 81-87.
38. Alexander, A., et al., Poly(ethylene glycol)–poly(lactic-co-glycolic acid) based thermosensitive injectable hydrogels for biomedical applications. Journal of Controlled Release, 2013. 172(3):
39. Lee, W.-F. and Y.-C. Chen, Effect of bentonite on the physical properties and drug-release behavior of poly(AA-co-PEGMEA)/bentonite nanocomposite hydrogels for mucoadhesive.
Journal of Applied Polymer Science, 2004. 91(5): p. 2934-2941.
40. Sohn, S.S., et al., Biomimetic and photo crosslinked hyaluronic acid/pluronic F127 hydrogels with enhanced mechanical and elastic properties to be applied in tissue engineering.
Macromolecular Research, 2016. 24(3): p. 282-291.
41. Lai, F. and H. Li, Modeling of effect of initial fixed charge density on smart hydrogel response to ionic strength of environmental solution. Soft Matter, 2010. 6(2): p. 311-320.
42. Bueno, V.B., et al., Synthesis and swelling behavior of xanthan-based hydrogels. Carbohydrate Polymers, 2013. 92(2): p. 1091-1099.
43. Serra, L., J. Doménech, and N.A. Peppas, Drug transport mechanisms and release kinetics from molecularly designed poly(acrylic acid-g-ethylene glycol) hydrogels. Biomaterials, 2006.
27(31): p. 5440-5451.
44. Kragh-Hansen, U., Molecular aspects of ligand binding to serum albumin. Pharmacol Rev, 1981. 33(1): p. 17-53.
45. Cevik, O., D. Gidon, and S. Kizilel, Visible-light-induced synthesis of pH-responsive composite hydrogels for controlled delivery of the anticonvulsant drug pregabalin. Acta Biomaterialia, 2015. 11: p. 151-161.
46. Chaturvedi, K., et al., Polymeric hydrogels for oral insulin delivery. Journal of Controlled Release, 2013. 165(2): p. 129-138.
47. Holt, J.K., et al., Fast Mass Transport Through Sub-2-Nanometer Carbon Nanotubes. Science, 2006. 312(5776): p. 1034-1037.
48. Thomas, J.A. and A.J.H. McGaughey, Reassessing Fast Water Transport Through Carbon Nanotubes. Nano Letters, 2008. 8(9): p. 2788-2793.
49. Hoffman, A.S., Hydrogels for biomedical applications. Advanced Drug Delivery Reviews, 2012. 64: p. 18-23.
50. Schexnailder, P. and G. Schmidt, Nanocomposite polymer hydrogels. Colloid and Polymer Science, 2009. 287(1): p. 1-11.
51. Dragan, E.S., Design and applications of interpenetrating polymer network hydrogels. A review.
Chemical Engineering Journal, 2014. 243: p. 572-590.
52. Hern, D.L. and J.A. Hubbell, Incorporation of adhesion peptides into nonadhesive hydrogels useful for tissue resurfacing. Journal of Biomedical Materials Research, 1998. 39(2): p. 266- 276.
53. Schmedlen, R.H., K.S. Masters, and J.L. West, Photocrosslinkable polyvinyl alcohol hydrogels that can be modified with cell adhesion peptides for use in tissue engineering. Biomaterials, 2002. 23(22): p. 4325-4332.
54. Nguyen, K.T. and J.L. West, Photopolymerizable hydrogels for tissue engineering applications.
Biomaterials, 2002. 23(22): p. 4307-4314.
55. Wenceslau, A.C., et al., Thermo- and pH-sensitive IPN hydrogels based on PNIPAAm and PVA- Ma networks with LCST tailored close to human body temperature. Materials Science and Engineering: C, 2012. 32(5): p. 1259-1265.
56. Cha, C., et al., Integrative design of a poly(ethylene glycol)-poly(propylene glycol)-alginate
hydrogel to control three dimensional biomineralization. Biomaterials, 2011. 32(11): p. 2695- 2703.
57. Zhao, X., et al., Photocrosslinkable Gelatin Hydrogel for Epidermal Tissue Engineering.
Advanced Healthcare Materials, 2016. 5(1): p. 108-118.
58. Nomura, Y., et al., Genotoxicity of dental resin polymerization initiators in vitro. Journal of Materials Science: Materials in Medicine, 2006. 17(1): p. 29-32.
59. Bail, R., et al., The Effect of a Type I Photoinitiator on Cure Kinetics and Cell Toxicity in Projection-Microstereolithography. Procedia CIRP, 2013. 5: p. 222-225.
60. Anseth, K.S., et al., In situ forming degradable networks and their application in tissue engineering and drug delivery. Journal of Controlled Release, 2002. 78(1): p. 199-209.
61. Li, Y., et al., In situ hydrogel constructed by starch-based nanoparticles via a Schiff base reaction. Carbohydrate Polymers, 2014. 110: p. 87-94.
62. Darling, N.J., et al., Controlling the kinetics of thiol-maleimide Michael-type addition gelation kinetics for the generation of homogenous poly(ethylene glycol) hydrogels. Biomaterials, 2016.
101: p. 199-206.
63. Zhu, H.-Z., et al., Click synthesis of hydrogels by metal-free 1,3-dipolar cycloaddition reaction between maleimide and azide functionalized polymers. Macromolecular Research, 2016. 24(9):
64. Choi, S.M., et al., Synthesis and characterization of in situ gellable poly(glycerol sebacate)-co- poly(ethylene glycol) polymers. Macromolecular Research, 2017. 25(1): p. 85-91.
65. Wang, J., et al., In Situ-Forming Polyamidoamine Dendrimer Hydrogels with Tunable Properties Prepared via Aza-Michael Addition Reaction. ACS Applied Materials & Interfaces, 2017. 9(12): p. 10494-10503.
66. Nguyen, Q.V., et al., Injectable polymeric hydrogels for the delivery of therapeutic agents: A review. European Polymer Journal, 2015. 72: p. 602-619.
67. Lutolf, M.P. and J.A. Hubbell, Synthesis and Physicochemical Characterization of End-Linked Poly(ethylene glycol)-co-peptide Hydrogels Formed by Michael-Type Addition.
Biomacromolecules, 2003. 4(3): p. 713-722.
68. Forrest, M.L., J.T. Koerber, and D.W. Pack, A Degradable Polyethylenimine Derivative with Low Toxicity for Highly Efficient Gene Delivery. Bioconjugate Chemistry, 2003. 14(5): p. 934- 940.
69. Pack, D.W., et al., Design and development of polymers for gene delivery. Nature Reviews Drug Discovery, 2005. 4(7): p. 581-593.
70. Hahn, M.S., J.S. Miller, and J.L. West, Three-Dimensional Biochemical and Biomechanical Patterning of Hydrogels for Guiding Cell Behavior. Advanced Materials, 2006. 18(20): p. 2679- 2684.
71. Liang, Y., et al., Tuning the non-equilibrium state of a drug-encapsulated poly(ethylene glycol) hydrogel for stem and progenitor cell mobilization. Biomaterials, 2011. 32(7): p. 2004-2012.
72. Zuidema, J.M., et al., A protocol for rheological characterization of hydrogels for tissue engineering strategies. Journal of Biomedical Materials Research Part B: Applied Biomaterials, 2014. 102(5): p. 1063-1073.
73. Weng, L., X. Chen, and W. Chen, Rheological Characterization of in Situ Crosslinkable Hydrogels Formulated from Oxidized Dextran and N-Carboxyethyl Chitosan.
Biomacromolecules, 2007. 8(4): p. 1109-1115.
74. Metters, A.T., C.N. Bowman, and K.S. Anseth, A Statistical Kinetic Model for the Bulk Degradation of PLA-b-PEG-b-PLA Hydrogel Networks. The Journal of Physical Chemistry B, 2000. 104(30): p. 7043-7049.
75. Lee, K., et al., Dual ionic crosslinked interpenetrating network of alginate-cellulose beads with enhanced mechanical properties for biocompatible encapsulation. Cellulose, 2017. 24(11): p.
76. Dash, S., et al., Kinetic modeling on drug release from controlled drug delivery systems. Acta Pol Pharm, 2010. 67(3): p. 217-23.
77. Ritger, P.L. and N.A. Peppas, A simple equation for description of solute release I. Fickian and non-fickian release from non-swellable devices in the form of slabs, spheres, cylinders or discs.
Journal of Controlled Release, 1987. 5(1): p. 23-36.
78. Piculell, L. and B. Lindman, Association and segregation in aqueous polymer/polymer, polymer/surfactant, and surfactant/surfactant mixtures: similarities and differences. Advances in Colloid and Interface Science, 1992. 41: p. 149-178.
79. Anseth, K.S., C.M. Wang, and C.N. Bowman, Reaction behaviour and kinetic constants for photopolymerizations of multi(meth)acrylate monomers. Polymer, 1994. 35(15): p. 3243-3250.
80. Pritchard, C.D., et al., An injectable thiol-acrylate poly(ethylene glycol) hydrogel for sustained release of methylprednisolone sodium succinate. Biomaterials, 2011. 32(2): p. 587-597.
81. Saito, H., A.S. Hoffman, and H.I. Ogawa, Delivery of Doxorubicin from Biodegradable PEG Hydrogels Having Schiff Base Linkages†. Journal of Bioactive and Compatible Polymers, 2007.
22(6): p. 589-601.
82. Malkoch, M., et al., Synthesis of well-defined hydrogel networks using Click chemistry.
Chemical Communications, 2006(26): p. 2774-2776.
83. Seliktar, D., Designing Cell-Compatible Hydrogels for Biomedical Applications. Science, 2012.
336(6085): p. 1124-1128.
84. Cha, C., et al., Designing Biomaterials To Direct Stem Cell Fate. ACS Nano, 2012. 6(11): p.
85. Loessner, D., et al., Bioengineered 3D platform to explore cell–ECM interactions and drug
resistance of epithelial ovarian cancer cells. Biomaterials, 2010. 31(32): p. 8494-8506.
86. Tibbitt, M.W. and K.S. Anseth, Hydrogels as extracellular matrix mimics for 3D cell culture.
Biotechnology and Bioengineering, 2009. 103(4): p. 655-663.
87. Mironi-Harpaz, I., et al., Photopolymerization of cell-encapsulating hydrogels: Crosslinking efficiency versus cytotoxicity. Acta Biomaterialia, 2012. 8(5): p. 1838-1848.
88. Temenoff, J.S., et al., In Vitro Cytotoxicity of Redox Radical Initiators for Cross-Linking of Oligo(poly(ethylene glycol) fumarate) Macromers. Biomacromolecules, 2003. 4(6): p. 1605- 1613.
89. Tromayer, M., et al., A biocompatible diazosulfonate initiator for direct encapsulation of human stem cells via two-photon polymerization. Polymer Chemistry, 2018. 9(22): p. 3108-3117.
90. Van Tomme, S.R., G. Storm, and W.E. Hennink, In situ gelling hydrogels for pharmaceutical and biomedical applications. International Journal of Pharmaceutics, 2008. 355(1): p. 1-18.
91. Yu, L. and J. Ding, Injectable hydrogels as unique biomedical materials. Chemical Society Reviews, 2008. 37(8): p. 1473-1481.
92. Metters, A. and J. Hubbell, Network Formation and Degradation Behavior of Hydrogels Formed by Michael-Type Addition Reactions. Biomacromolecules, 2005. 6(1): p. 290-301.
93. Jang, J. and C. Cha, Multivalent Polyaspartamide Cross-Linker for Engineering Cell- Responsive Hydrogels with Degradation Behavior and Tunable Physical Properties.
Biomacromolecules, 2018. 19(2): p. 691-700.
94. Kim, M. and C. Cha, Integrative control of mechanical and degradation properties of in situ crosslinkable polyamine-based hydrogels for dual-mode drug release kinetics. Polymer, 2018.
145: p. 272-280.
95. Kim, M. and C. Cha, Modulation of functional pendant chains within poly (ethylene glycol) hydrogels for refined control of protein release. Scientific reports, 2018. 8(1): p. 1-12.
96. Tan, H., et al., Injectable in situ forming biodegradable chitosan–hyaluronic acid based hydrogels for cartilage tissue engineering. Biomaterials, 2009. 30(13): p. 2499-2506.
97. Liu, Y., et al., Preparation of therapeutic-laden konjac hydrogel for tumor combination therapy.
Chemical Engineering Journal, 2019. 375: p. 122048.
98. Wu, C., et al., Design of injectable agar-based composite hydrogel for multi-mode tumor therapy. Carbohydrate Polymers, 2018. 180: p. 112-121.
99. Zheng, Y., et al., Preparation of injectable temperature-sensitive chitosan-based hydrogel for combined hyperthermia and chemotherapy of colon cancer. Carbohydrate Polymers, 2019. 222:
100. Bonino, C.A., et al., Real-time in siturheology of alginate hydrogel photocrosslinking. Soft Matter, 2011. 7(24): p. 11510-11517.
101. Berger, J., et al., Structure and interactions in covalently and ionically crosslinked chitosan
hydrogels for biomedical applications. European Journal of Pharmaceutics and Biopharmaceutics, 2004. 57(1): p. 19-34.
102. Bhattarai, N., J. Gunn, and M. Zhang, Chitosan-based hydrogels for controlled, localized drug delivery. Advanced Drug Delivery Reviews, 2010. 62(1): p. 83-99.
103. Chung, H. and R.H. Grubbs, Rapidly Cross-Linkable DOPA Containing Terpolymer Adhesives and PEG-Based Cross-Linkers for Biomedical Applications. Macromolecules, 2012. 45(24): p.
104. Qu, J., et al., Antibacterial adhesive injectable hydrogels with rapid self-healing, extensibility and compressibility as wound dressing for joints skin wound healing. Biomaterials, 2018. 183:
105. Alves, N.M. and J.F. Mano, Chitosan derivatives obtained by chemical modifications for biomedical and environmental applications. International Journal of Biological Macromolecules, 2008. 43(5): p. 401-414.
106. Islas, L., G. Burillo, and A. Ortega, Graft Copolymerization of 2-Hydroxyethyl Methacrylate onto Chitosan Using Radiation Technique for Release of Diclofenac. Macromolecular Research, 2018. 26(8): p. 690-695.
107. Bhattarai, N., et al., PEG-grafted chitosan as an injectable thermosensitive hydrogel for sustained protein release. Journal of Controlled Release, 2005. 103(3): p. 609-624.
108. Harris, J.M., et al., Synthesis and characterization of poly(ethylene glycol) derivatives. Journal of Polymer Science: Polymer Chemistry Edition, 1984. 22(2): p. 341-352.
109. Hong, J., et al., Complex Tuning of Physical Properties of Hyperbranched Polyglycerol-Based Bioink for Microfabrication of Cell-Laden Hydrogels. Advanced Functional Materials, 2019.
29(13): p. 1808750.
110. Lih, E., et al., Rapidly curable chitosan–PEG hydrogels as tissue adhesives for hemostasis and wound healing. Acta Biomaterialia, 2012. 8(9): p. 3261-3269.
111. Strehin, I., et al., A versatile pH sensitive chondroitin sulfate–PEG tissue adhesive and hydrogel.
Biomaterials, 2010. 31(10): p. 2788-2797.
112. Zhang, H., et al., Mussel-inspired hyperbranched poly(amino ester) polymer as strong wet tissue adhesive. Biomaterials, 2014. 35(2): p. 711-719.
113. Assmann, A., et al., A highly adhesive and naturally derived sealant. Biomaterials, 2017. 140:
114. Vuocolo, T., et al., A Highly Elastic and Adhesive Gelatin Tissue Sealant for Gastrointestinal Surgery and Colon Anastomosis. Journal of Gastrointestinal Surgery, 2012. 16(4): p. 744-752.
115. Barua, S., P. Chattopadhyay, and N. Karak, s-Triazine-based biocompatible hyperbranched epoxy adhesive with antibacterial attributes for sutureless surgical sealing. Journal of Materials Chemistry B, 2015. 3(28): p. 5877-5885.
116. Askaruly, S., et al., Quantitative Evaluation of Skin Surface Roughness Using Optical Coherence Tomography In Vivo. IEEE Journal of Selected Topics in Quantum Electronics, 2019.
25(1): p. 1-8.
117. Choi, G., et al., Image‐guided recording system for spatial and temporal mapping of neuronal activities in brain slice. Journal of biophotonics, 2018. 11(3): p. e201700243.
118. Wiegand, I., K. Hilpert, and R.E.W. Hancock, Agar and broth dilution methods to determine the minimal inhibitory concentration (MIC) of antimicrobial substances. Nature Protocols, 2008. 3: p. 163.
119. Balouiri, M., M. Sadiki, and S.K. Ibnsouda, Methods for in vitro evaluating antimicrobial activity: A review. Journal of Pharmaceutical Analysis, 2016. 6(2): p. 71-79.
120. Dash, M., et al., Chitosan—A versatile semi-synthetic polymer in biomedical applications.
Progress in Polymer Science, 2011. 36(8): p. 981-1014.
121. Jang, Y., et al., Interfacial Compression-Dependent Merging of Two Miscible Microdroplets in an Asymmetric Cross-Junction for In Situ Microgel Formation. Macromolecular Research, 2018. 26(12): p. 1143-1149.
122. Qu, J., et al., pH-responsive self-healing injectable hydrogel based on N-carboxyethyl chitosan for hepatocellular carcinoma therapy. Acta Biomaterialia, 2017. 58: p. 168-180.
123. Pielichowski, K. and K. Flejtuch, Differential scanning calorimetry studies on poly(ethylene glycol) with different molecular weights for thermal energy storage materials. Polymers for Advanced Technologies, 2002. 13(10‐12): p. 690-696.
124. Berezkin, A.V. and Y.V. Kudryavtsev, Effect of Cross-Linking on the Structure and Growth of Polymer Films Prepared by Interfacial Polymerization. Langmuir, 2015. 31(44): p. 12279- 12290.
125. Liu, N.C., G.P. Yao, and H. Huang, Influences of grafting formulations and processing conditions on properties of silane grafted moisture crosslinked polypropylenes. Polymer, 2000.
41(12): p. 4537-4542.
126. Wang, B., et al., Copolymerization of propylene with Si-containing α,ω-diolefins: how steric hindrance of diolefins affects long chain branch formation. Polymer Chemistry, 2016. 7(17): p.
127. Hozumi, T., et al., Injectable Hydrogel with Slow Degradability Composed of Gelatin and Hyaluronic Acid Cross-Linked by Schiff’s Base Formation. Biomacromolecules, 2018. 19(2):
128. Kong, H.J., et al., Controlling Degradation of Hydrogels via the Size of Crosslinked Junctions.
Advanced Materials, 2004. 16(21): p. 1917-1921.
129. Etemadi, H., R. Yegani, and M. Seyfollahi, The effect of amino functionalized and polyethylene glycol grafted nanodiamond on anti-biofouling properties of cellulose acetate membrane in
membrane bioreactor systems. Separation and Purification Technology, 2017. 177: p. 350-362.
130. Jayakumar, R., et al., Biomaterials based on chitin and chitosan in wound dressing applications.
Biotechnology Advances, 2011. 29(3): p. 322-337.
131. Kroez, M., W. Lang, and G. Dickneite, Wound healing and degradation of the fibrin sealant Beriplast® P following partial liver resection in rabbits. Wound Repair and Regeneration, 2005.
13(3): p. 318-323.
132. Alemdaroğlu, C., et al., An investigation on burn wound healing in rats with chitosan gel formulation containing epidermal growth factor. Burns, 2006. 32(3): p. 319-327.
133. Field, C.K. and M.D. Kerstein, Overview of wound healing in a moist environment. The American Journal of Surgery, 1994. 167(1, Supplement): p. S2-S6.
134. Siepmann, J. and F. Siepmann, Modeling of diffusion controlled drug delivery. Journal of Controlled Release, 2012. 161(2): p. 351-362.
135. Kim, S.W., Y.H. Bae, and T. Okano, Hydrogels: Swelling, Drug Loading, and Release.
Pharmaceutical Research, 1992. 9(3): p. 283-290.
136. Top, A. and K.L. Kiick, Multivalent protein polymers with controlled chemical and physical properties. Advanced Drug Delivery Reviews, 2010. 62(15): p. 1530-1540.
137. Hacker, M.C. and H.A. Nawaz, Multi-Functional Macromers for Hydrogel Design in Biomedical Engineering and Regenerative Medicine. International Journal of Molecular Sciences, 2015. 16(11): p. 27677-27706.
138. Jalalvandi, E. and A. Shavandi, Polysuccinimide and its derivatives: Degradable and water soluble polymers (review). European Polymer Journal, 2018. 109: p. 43-54.
139. Nakato, T., A. Kusuno, and T. Kakuchi, Synthesis of poly(succinimide) by bulk polycondensation of L-aspartic acid with an acid catalyst. Journal of Polymer Science Part A:
Polymer Chemistry, 2000. 38(1): p. 117-122.
140. Roweton, S., S.J. Huang, and G. Swift, Poly(aspartic acid): Synthesis, biodegradation, and current applications. Journal of environmental polymer degradation, 1997. 5(3): p. 175-181.
141. Tomida, M., et al., Convenient synthesis of high molecular weight poly(succinimide) by acid- catalysed polycondensation of l-aspartic acid. Polymer, 1997. 38(18): p. 4733-4736.
142. Pitarresi, G., et al., Biodegradable hydrogels obtained by photocrosslinking of dextran and polyaspartamide derivatives. Biomaterials, 2003. 24(23): p. 4301-4313.
143. Tran, N.B., et al., CO2-responsive swelling behavior and metal-ion adsorption properties in novel histamine-conjugated polyaspartamide hydrogel. Journal of Applied Polymer Science, 2016. 133(16).
144. Wang, B., et al., Self-healable mussel-mimetic nanocomposite hydrogel based on catechol- containing polyaspartamide and graphene oxide. Materials Science and Engineering: C, 2016.
69: p. 160-170.